Swipe to navigate through the chapters of this book
The limited supply of bone graft is a major problem in human organ transplantation costing lives of many worldwide. Calcium phosphate (CaP) material has been considered the most favorable and best substitute in tissue engineering and orthopedics, thanks to its good biocompatibility and osteoconductivity. However, one of disadvantages of this material is its limited clinical applications for non-load-bearing bone implant due to low strength and brittleness. The objective of this study was to develop high mechanical strength calcium phosphate ceramics mechanically suitable for load-bearing bone implant application. Chemical and physical approaches have been undertaken to solve the mechanical weakness of calcium phosphate ceramics by doping with zinc (Zn) and compositing with carbon nanotube (CNT), respectively. The starting powders have been synthesized via sol-gel method. After uniaxial pressing, the compacted samples were sintered using conventional pressureless sintering. The samples were studied in terms of the phase stability, relative density, Vickers hardness, fracture toughness as well as in vitro test in SBF solution. The results showed that hydroxyapatite is the main phase and β-tricalcium phosphate is the secondary phase of obtained powders. The composites have relative density 93.34 ± 0.50% with a Vickers hardness as high as 5.00 ± 0.02 GPa and 2.78 ± 0.01 MPa.m1/2 fracture toughness, which are in the range of human cortical bone’s mechanical properties. Bioactivity test in a simulated body fluid for 1, 7, 14 and 30 days showed that the samples were covered by apatite cell since the first day, and the density of apatite increased by immersion time. Thus, from mechanical and bioactivity characteristic viewpoint, this CNT reinforced Zn-doped calcium phosphate is mechanically and biologically suitable for load-bearing bone implant applications.
Please log in to get access to this content
To get access to this content you need the following product:
Ku S.H.; Lee M.; Park C.B. Carbon-based nomaterials for tissue engineering, Advanced healthcare materials 2013, 2 (2), 244–260.
Dubin R.A.; Callegari G.C.; Kohn J.; Neimark A.V. Carbon nanotube fibers are compatible with mammalian cells and neurons, IEEE Transactions on Nanobiosciense 2008, 7 (1), 11–14.
Chao T.I.; Xiang S.; Chen C.S.; Chin W.C.; Nelson A.J.; Wang C.; Lu J. Carbon nanotubes promote neuron differentiation from human embryonic stem cells, Biochemical Biophysical Reseach Communications 2009, 384 (4), 426–430.
Dorozhkin S.V. Biphasic, triphasic and multiphasic calcium orthophosphates, Acta Biomaterialia 2012, 8 (3), 963–977.
Daculsi G.; Laboux O.; Malard O.; Weiss P. Current state of the art of biphasic calcium phosphate bioceramics, Journal of Materials Science: Materials in Medicine 2003, 14 (3), 195–200.
Chen Y.; Miao X. Effect of fluorine addition on the corrosion resistance of hydroxyapatite ceramics, Ceramics International 2004, 30 (7), 1961–1965.
Jiao M.J.; Wang X.X. Electrolytic deposition of magnesium-substituted hydroxyapatite crystals on titanium substrate, Materials Letters 2009, 63 (27), 2286–2289.
Yamaguchi M.; Oishi H.; Suketa Y. Stimulatory effect of zinc on bone formation in tissue culture, Biochemical Pharmacology 1987, 36 (22), 4007–4012.
Ito A.; Otsuka M.; Kawamura H.; Ikeuchi M.; Ohgushi H.; Sogo Y.; Ichinose N. Zinc-containing tricalcium phosphate and related materials for promoting bone formation, Current Applied Physics 2005, 5 (5), 402–406.
Yamaguchi M. Nutritional factors and bone homeostasis: synergistic effect with zinc and genistein in osteogenesis, Molecular and cellular biochemistry 2012, 366 (1–2), 201-221.
Ramesh S.; Tan C.Y.; Tolouei R.; Amiriyan M.; Purbolaksono J.; Sopyan I.; Teng W.D. Sintering behavior of hydroxyapatite prepared from different routes, Materials & Design 2012, 34, 148–154.
Wang X.; Nyman J.S.; Dong X.; Leng H.; Reyes M. Fundamental biomechanics in bone tissue engineering: Morgan & Claypool; 2010.
Shin U.S.; Yoon I.K.; Lee G.S.; Jang W.C.; Knowles J.C.; Kim H.W. Carbon nanotubes in nanocomposites and hybrids with hydroxyapatite for bone replacements, Journal of Tissue Engineering 2011, 2011, 1–10.
White A.A.; Kinloch I.A.; Windle A.H.; Best S.M. Optimization of the sintering atmosphere for high-density hydroxyapatite-carbon nanotube composites, Journal of The Royal Society Interface 2010, 7 Suppl 5, 1–11.
Zhao L.; Gao L. Novel in situ synthesis of MWNTs-hydroxyapatite composites, Carbon 2004, 42 (2), 423–426.
Neelgund G.M.; Olurode K.; Oki A. A simple and rapid method to graft hydroxyapatite on carbon nanotubes, Materials Science and Engineering C 2011, 31 (7), 1477–1481.
Osorio A.G.; dos Santos L.A.; Bergmann C.P. Evaluation of the Mechanical Properties and Microstructure of Hydroxyapatite Reinforced with Carbon Nanotubes, Review on Advance Materials Science 2011, 27, 58–63.
Gunawan; Sopyan I.; Suryanto; Naqshbandi A. Zinc-doped biphasic calcium phosphate nanopowders synthesized via sol-gel method, Indian Journal of Chemistry Section a-Inorganic Bio-Inorganic Physical Theoretical & Analytical Chemistry 2014, 54A, 152–158.
Bezzi G.; Celotti G.; Landi E.; La Torretta T.M.G.; Sopyan I.; Tampieri A. A novel sol-gel technique for hydroxyapatite preparation, Materials Chemistry and Physics 2003, 78 (3), 816–824.
Niihara K. Indentation microfracture of ceramics—its application and problems, Journal of the Ceramic Society of Japan 1985, 20, 12–18.
Wang C.K.; Ju C.P.; Chem Lin J.H. Effect of doped bioactive glass on structure and properties of sintered hydroxyapatite, Materials Chemistry and Physics 1998, 53, 138–149.
Kokubo T.; Takadama H. How useful is SBF in predicting in vivo bone bioactivity?, Biomaterials 2006, 27 (15), 2907–2915.
- Calcium Phosphate-Carbon Nanotube Composites for Load—Bearing Bone Implant Application
- Springer Singapore
- Sequence number